Twolevel states in glasses


 Everett Fleming
 1 years ago
 Views:
Transcription
1 Rep. Prog. Phys. 50 (1987) Printed in the UK Twolevel states in glasses W A Phillips Cavendish Laboratory, University of Cambridge, Madingley Road, Cambridge CB3 OHE, UK Abstract This review covers a wide range of experimental and theoretical studies of twolevel or tunnelling states in glasses. Emphasis is on fundamental physics rather than a detailed comparison of experiment and theory. Sections cover the static and dynamic properties of tunnelling states, their contribution to thermal properties and their response to weak and strong electric and acoustic fields, both steady state and pulsed. A section on metallic glasses focuses on the importance of electron tunnellingstate interactions, and a final section illustrates approaches to a microscopic description by means of selected examples. This review was received in February /87/ IOP Publishing Ltd 1657
2 1658 W A Phillips Contents 1, Introduction 2. Tunnelling states 2.1. Static description 2.2. Dynamics 3. Thermal properties 3.1. Thermal conductivity 3.2. Heat capacity 3.3. Thermal expansion 3.4. Energy relaxation and irreversibility 4. Response to external fields 4.1. Weak fields 4.2. Strong fields 4.3. Relaxation 5. Pulse echo experiments 5.1. General theory 5.2. Echo experiments 5.3. Spectral diffusion 6. Metallic glasses 7. Microscopic descriptions of tunnelling states 7.1. Relation to specific defects 7.2. Microscopic modelling 7.3. General theories 7.4. suffix Acknowledgments References Page
3 Twolevel states in glasses Introduction One of the more unexpected results in solid state physics was provided by the first reliable measurements below 1 K of heat capacity C and thermal conductivity K in a number of glasses (Zeller and Pohl 1971). Beforehand it had been argued that because lowtemperature thermal properties are dominated by phonons (quantised lattice vibrations) of low frequency, and because in crystals these phonons can be described as longwavelength sound waves propagating through an elastic continuum, there should be little difference between glasses and crystals in this regime where the phonons are insensitive to microscopic structure. In fact, as shown in figures 1 and 2 for vitreous and crystalline silica, the heat capacity and thermal conductivity are radically different in the two materials. \ Vitreous silica \ \ \ \ T IKI Figure 1. The heat capacity C( T) of vitreous silica and crystalline quartz as a function of temperature T (Jones 1982, after Zeller and Pohl 1971), plotted as C/T3 against T The results in aquartz are typical of an insulating crystal. The heat capacity varies as T3 below 10 K, where T is the absolute temperature, as expected from the Debye theory. This theory predicts that in the longwavelength limit the density of phonon states g(w) varies quadratically with the phonon (angular) frequency w if the velocity of sound U, is constant so that wq = v,,, where q is the phonon wavevector. At higher temperatures phonon dispersion initially gives a more rapid increase of g(w) with w, and so C increases more rapidly than T3, but ultimately, above the Debye temperature 0, C approaches the classical limit. The cubic temperature variation of K can be interpreted qualitatively by means of the kinetic formula K =fcv,l (1.1)
4 1660 W A Phillips 102 IO lo T ik1 Figure 2. The thermal conductivity K(T) of vitreous silica and crystalline quartz (Jones 1982, after Zeller and Pohl 1971), plotted logarithmically. where 1 is the phonon mean free path. At low temperatures phonons are scattered by defects in the crystal or by the surfaces of the sample, so that 1 is independent of temperature and K is therefore proportional to T3. Above 40 K the reduction of 1 by phononphonon scattering leads to the peak and subsequent fall in K. These ideas are well known and serve to emphasise the peculiarity of the results in vitreous silica, where C varies approximately as T and at 0.1 K is about two orders of magnitude greater in the glass than in the crystal. Below 1 K K varies as T19 but varies only slightly with temperature between 4 and 20 K before increasing at high temperatures to a value approaching that of crystalline quartz. Similar results are seen in a wide range of other amorphous solids; oxide, chalcogenide, elemental, polymeric and metallic glasses all show the same behaviour. A representative sample is shown in figures 3 and 4. The universality of the phenomena and the idealised temperature dependences of C proportional to T and K proportional to T proved great attractions for theorists. In retrospect this idealisation can be seen to have handicapped the search for a theoretical explanation, suggesting as it did very general models which were not supported by a detailed examination of the experimental results and which were ultimately unable to give quantitative agreement with experiment. For example, the first and perhaps most obvious explanation for C was in terms of electron states (Redfield 1971). In the amorphous state the sharp distinction between energy gaps
5 Twolevel states in glasses I I I I T2 ikz) Figure 3. C( T)/ T plotted as a function of T2 for a range of glasses (Stephens 1973). and energy bands can be blurred by disorder, and it was suggested that the specific heat was a result of an almost constant density of states at the Fermi level, giving a linear variation of C with T just as in a metal. However, it turns out that the density of states estimated from optical experiments (less than J' m3 or lo'* ev' cm') is much smaller than that deduced from the heat capacity ( J' m')). Similar quantitative problems arise in a model for thermal conductivity based on the scattering of sound waves by inhomogeneities in the glass structure, a form of Rayleigh scattering by variations in the local velocity of sound. In this case the magnitude of density fluctuations estimated thermodynamically or from light scattering experiments is too small to give significant scattering below 1 K, and although there is no independent way of directly estimating the local variation in velocity, the required magnitude is unreasonably large (Jones e? a1 1978). Sound waves are known to exist in glasses. In addition to measurements of the velocity of sound, limited to frequencies below about 1 GHz, evidence for the existence of well defined transverse and longitudinal waves comes from Brillouin scattering below 30 GHz (Vacher and Pelous 1976) and phonon interference experiments (Rothenfusser et a1 1983) up to 500GHz in vitreous silica. Consistent velocities are
6 1662 W A Phillips Figure 4. K( T) as a function of temperature for a range of glasses (Stephens 1973). measured in all these experiments, and the phonon mean free path is much greater than the wavelength. Further evidence is provided by measurements of thermal conductivity in very thin glass rods which have roughened surfaces to ensure that boundary scattering dominates (Pohl er a1 1974, Zaitlin and Anderson 1975). Experimental values agree with those calculated assuming the existence of sound waves. It is clear, therefore, that the unexpected thermal properties arise from additional excitations which both scatter phonons and contribute to the heat capacity. Of the various models originally proposed to account for the thermal data, the one most widely and successfully used has been the tunnelling or twolevelsystem model (Phillips 1972, Anderson et a1 1972). In this model, to be described in detail in the next section, atoms occupying one of two adjacent minima are assumed to tunnel quantum mechanically to the other, leading to a splitting of the ground state as in the ammonia molecule. The inevitable variations in local environment present in the amorphous solid give rise to a distribution of these splittings which is almost constant in energy, and hence to a heat capacity which can be evaluated as I: C(T) = n0(e2/4kbt2) sech2(e/2kbt) de (12) where no is the constant density of states and the other factor in the integrand is the contribution of a single twolevel state (Schottky anomaly). Evaluating the integral gives C(T)=(~ /6)nokg~T (1.3)
7 Twolevel states in glasses 1663 in broad agreement with experiment. These states scatter phonons, leading to a thermal conductivity proportional to T2 and to an acoustic attenuation which can be saturated at high acoustic intensities. It is this last property that provides the strongest evidence for the model which will form the basis for the interpretation of the wide range of experimental results discussed in this review. To a large extent the model can be used in phenomenological form, and possible microscopic representations will be described only in the last section. This review is not intended as a detailed evaluation and comparison of experimental results in specific glasses, but as a critical description of the way in which the tunnelling or twolevelsystem model can be used to explain a wide range of data. By far the largest number of experiments have been performed on vitreous silica, and this material will be used as a running example, although reference will be made to other materials when necessary. 2. Tunnelling states 2.1. Static description In a perfect crystal each atom is constrained by symmetry to occupy a single potential minimum. Many defects, however, can be represented microscopically as interstitial or substitutional impurity atoms or molecules moving in a multiminima potential provided by the neighbours. Such states have been extensively studied in, for example, alkali halides (Narayanamurti and Pohl 1970). At low temperatures a quantum mechanical description is necessary, and tunnelling of the atom from one minimum to another gives rise to the very small energy splittings (less than ev) needed if the states are to be observed in thermal experiments at 1 K and below. The tunnelling model proposes that similar states are intrinsic to glasses: an atom or group of atoms can occupy one of two (or more) potential minima. This choice at the microscopic level is consistent with the experimentally determined excess entropy of the glass with respect to the crystal, although the number of atoms contributing at low temperatures is only a small fraction of the total. The remainder are essentially immobile below the glasstransition temperature Tg. Each tunnelling state (TS) can be represented by a particle in a potential of the form shown in figure 5(a), where the abscissa may represent the position of one atom but more generally is a configurational coordinate describing a combination of the coordinates of a number of atoms. The energy levels of the particle are conveniently calculated using as a starting point the solutions of the singlewell problem, a choice of basis set 41 and d2 known as the well, nondiagonal or localised representation (figure S(b)). Each state is the ground state of the appropriate potential Vl or V, (assumed harmonic in figure 5). The complete Hamiltonian H can be written as H = HI + ( v  v, ) = Hz + ( v  V2) (2.1) where HI and H2 are the individual well Hamiltonians. In the localised representation the Hamiltonian matrix becomes If the extension of each localised wavefunction into the barrier is small, the terms (4il V V,14i) can be neglected in comparison to Ei, and if the zero of energy is chosen
8 1664 W A Phillips Figure 5. A doublewell potential (a), together with the wavefunctions in the localised (b) and diagonal (c) representations. as the mean of E, and E*, (2.2) becomes where the tunnel splitting A, is given by (2.3) A,= 2{4llf442)* (2.4) Notice that only if the wells are identical, apart from a relative shift in energy, is the A of (2.3) identical to that of figure 5(a). A, can be evaluated for specific potentials: two overlapping harmonic potentials in two and three dimensions (Mertzbacker 1970, Phillips 1981b) and Mathieu s equation for a rigid rotator in twofold and threefold potentials (Isnard and Gilchrist 1981) are typical examples. The results all imply a similar exponential dependence of A, on the barrier height and well separation, although precise numerical values change from one model to another. The use of a particular detailed form cannot be justified in amorphous solids (as opposed to crystals) because the microscopic picture is uncertain, and so a simplified expression is usually adequate: A,= hr ea = ha exp[d(2mv,/h2) *] (2.5) where hr is approximately equal to (E, + E2)/2, d is the separation and V, the barrier between the two wells, and m is the particle mass. Typical values of the tunnelling parameter A can be estimated from the requirement that A, must be approximately equal to kbt if the tunnelling state is to contribute to
9 Twolevel states in glasses 1665 thermal properties at a temperature T. At 1 K this requires a tunnel splitting of ev, which with hr equal to ev gives approximately 5 for A. This is equivalent to a bare proton tunnelling across a barrier of 0.1 ev with d = 0.7 A. The matrix (2.3) can be diagonalized to obtain the eigenstates, the true, diagonal or energy representation. These eigenfunctions, illustrated in figure 5, have energies *El2 where E =(A2+A~)1 2 (2.6) and can be written in the analytic forms 9, = cos 0+42 sin 0 (2.7) ~2=~1sinO~,cos0 (2.8) where tan 20=A,/A. In the symmetric case where A=O these equations give the expected symmetric and antisymmetric solutions. The I dipole moment of the tunnelling state can be written in terms of G1 and I,!J2 as PI = 9Tqx*1 dx = q [ (4Tx41 cos 0 + 4Tx4, sin2 O+ 47~4~ sin 20) dx if the term involving 4Tx42 can be neglected, and where po is the dipole moment when the particle is located in one well: po = [ I 4Tx4, dx =  4$x42 dx. Obviously p1 is zero for the symmetric case. For this, as for any problem involving two energy levels, there is a formal analogy with the problem of a spin; particle in a magnetic field. The Hamiltonian matrix (2.3) can therefore be rewritten in terms of the Pauli spin matrices (2.10) (or equivalently in terms of the spin operators S, =+ha,). After diagonalisation, the Hamiltonian takes the obvious form H =$EuZ. This analogy has important advantages when discussing nonlinear and coherent effects in the interaction of tunnelling states with acoustic and electric fields ( 5). A basic feature of the tunnelling state model as applied to amorphous solids is the existence of a wide range of values of both the tunnelling parameter A and the asymmetry A. Calculated properties of the states will depend critically on the form of the distribution function f(a, A,) for A and Ao, the latter distribution derived from that for A. In the case of the asymmetry A it is argued that the distribution function must be symmetric because both positive and negative values of A are equally likely. (No singularities are expected for A = 0 because the eigenstates remain nondegenerate.) The scale of energy variation is determined by the thermal energy available at the
10 1666 W A Phillips glasstransition temperature where the fluctuating local potentials of the liquid are frozen in the structure, Since Tg is between 200 and 1OOOK for most glasses, this energy is of the order of 0.05 ev, much larger than the thermal energy available at 1 K. The low temperature properties are therefore sensitive to the centre of a broad symmetric distribution, so that f(a, A,) can be taken as independent of A. The variation with A, is likely to be sensitive to the particular microscopic motion involved, although the general form can be deduced from the distribution of the tunnelling parameter A. Because of the exponential dependence of A, on A, only a relatively small range of A is sampled for a large range of A, and over this limited range the distribution of A can be assumed constant. The resulting distribution function can then be written f(a, A,) = P/AO. (2.11) This general result is only slightly modified (by a logarithmic factor) if the distribution of A varies slowly with the energy, but in general the precise dependence on A. will vary from one material to another, and can be regarded as a parameter to be determined by experiment (Frossatti et a1 1977, Phillips 1981b). The density of states n(e) can be calculated from (2.6) and the distribution function f(a, A,) only if a lower cutoff value for A, is introduced when integrating (2.11). Such a cutoff could arise from a maximum tunnelling parameter (Lasjaunias et a1 1978) or from characteristic time scales introduced by experiment. More precisely, the two parameters A and A. describing the states must be replaced by a second pair of parameters, often chosen as the energy E and the relaxation time T. The resulting distribution function for E and T will be derived in 0 3. In many cases the results of experiment can be interpreted and related in terms of a simpler model which ignores the detailed origin of the two levels. Instead, of two parameters A and A,, this twolevelsystem model considers the total energy E as the only variable. The distribution function is assumed to be constant. Although in many cases it is clear that the twolevelsystem model is inadequate for detailed understanding, in others the simplification introduced by its use is very helpful Dynamics The behaviour of a tunnelling state is defined by specifying the complex amplitudes a,(t) and a,(t) of the two lowest states with eigenfunctions $,(r) and $*(r). Neglect of higher states is justified because these two states are much closer in energy to each other than they are to other excited states, although the possibility that higher energy states might be important must be considered in certain cases (such as transition rates at temperatures above 1 K). The general timedependent wavefunction takes the form V(r, t) =a,(t)$l(r) exp(ie,t/a)+a,(t)$,(r) exp(ie,t/h) (2.12) where E, and E2 are the energies of states $, and $z and for normalisation alat+ a2at = 1. The complex nature of a, and a2 means that two quantities are necessary to define the twolevel system, normally taken as the difference in probabilities of finding the system in the two states, a2a~a,u~, and a quantity related to the phase difference between a, and a2, ala$. Measurable properties of the system depend on these two parameters, as can be seen for example by calculating the timedependent dipole
11 Twolevel states in glasses 1667 moment of a onedimensional tunnelling state. Using p, = p2 = ( $,IX~$~) and p12 = p2, = ($llx[i,b2), the average dipole moment (p( t)) can be written where hwo = E2  E,. Variations of a,( t) and a2( t) are determined through the timedependent Schrodinger equation by interaction with external fields. Any twolevel system in a solid will be subject to randomly varying strain fields which can be treated as the superposition of independent phonon modes. The strain field of each is weak, and interaction with the two levels can be treated using perturbation theory, ignoring phase coherence, equivalent to the interaction of an atom with electromagnetic radiation in a blackbody cavity (Phillips 1981b). Experimentally the properties of the states may be probed by strong external applied electromagnetic or strain fields where coherence of the two wavefunctions I,bl and I,b2 must be taken into account, although for weak external fields perturbation theory can still be used. Two related simplifications can be made. The frequency needed to induce resonant transitions from one level to the other is less than 20GHz for states contributing to thermal properties below 1 K. Corresponding wavelengths are 10 mm for photons and 100 nm for acoustic phonons, in both cases much larger than the spatial extent of the tunnelling or twolevel state. The dipole approximation, where the local electric or strain field is taken as uniform, is therefore valid. The dominant effect of these uniform fields is to affect the energy of the tunnelling state by changing the asymmetry energy, and changes in the barrier height can usually be ignored (Phillips 1981b, Anderson 1986). Any external perturbation is therefore diagonal in the local representation ( 41, &) which when transformed into the diagonal representation ( $1, $2) has the form cos24 sin24 l : : l sin24 cos24 In terms of the Pauli matrices the general interaction Hamiltonian can be written Hint= uz+ux l : : l (2.14) po*&+ uz+ux ye (2.15) in the presence of an electric field 5 and a strain field e. The two parameters po and y, defined as fda/dg and ;aa/ae respectively, are equivalent to the electric and elastic dipole moments of the equivalent classical problem of a charged particle moving in the double well potential. In (2.15) the vector character of is preserved, but the tensorial nature of e has been ignored and ye written as an average over orientations. For the twolevelsystem model (2.15) must be replaced by an equivalent form for Hint in which the relationship between the diagonal (uz) and offdiagonal (ux) terms is ignored. In this model (2.15) is usually written Hint= (t~u,+~ ux)5+(tduz+mux)e. (2.16) In the remainder of this section the phase coherence of I,b, and I,b2 will be ignored in a calculation valid for interaction with thermal phonons and weak external fields. The only relevant parameter is therefore the occupation probability p, = alar, with p1 +p2 = 1. Using a rateequation approach (Golding and Graebner 1981) P1= PIwl2+P2w2I (2.17) li2 =PIw12p2~12 (2.18)
12 1668 W A Phillips where wi2 is the transition probability from state 1 to state 2. In thermal equilibrium at temperature T, p1 and p2 are time independent, with values py and p:, so that where P h 2 = P b21 p:lp?= exp(elkt) = wi2lw2, (2.19) if E is the energy difference between the two levels. Replacing p2 in (2.17) gives $1 = PI(Wlr+ w21) + U 21 (2.20) defining a relaxation time T, where 1 T =(w12+w21)=w,2[1+exp (ElkT)]. (2.21) This relaxation time refers to the occupation probabilities, and so governs the relaxation of the term ala?  a2a; in the expression for (p) in (2.13). To distinguish it from the relaxation time for terms of the form ala: (see 0 4.2) it is often referred to as TI, or the spinlattice relaxation time. The transition probability can be calculated for a weak strain field using timedependent perturbation theory to give (2.22) where nb, the Bose factor, is [exp(e/kt)  l]', g(e) is the phonon density of states, and the summation is over phonon polarisations a. For an acoustic wave 2e, cos of the strain amplitude per phonon is given by equating the time average classical energy per unit volume to the energy of a phonon: 2pu2w2 = ho where U is the displacement amplitude and p is the bulk density. The strain is given by (2.23) where qa is the phonon wavevector, and the matrix element, using the term in ax in Hint (a, gives nothing), becomes 1/2 The Debye density of phonon states, valid in this lowenergy limit, is (2.24) g(e) = E2/2.rr2h3vi (2.25) per unit volume, where U, is the sound velocity for polarisation a. Collecting together (2.21), (2.22) and (2.24) gives (2.26) In the equivalent result for the twolevel system Ai is replaced by E', but it should be noted that this removes the very wide range of relaxation times predicted by (2.26) through the broad distribution of A,, and found experimentally ( At higher temperatures additional higherorder processes will of course contribute 1 o relaxation, but these have not been clearly observed in glasses.
13 3. Thermal properties 3.1. Thermal conductivity Twolevel states in glasses 1669 The interaction between TS and phonons reduces the phonon mean free path, and is the dominant scattering mechanism in glasses below 1 K. An expression for the free path, valid for weak fields (see 4) can be obtained from the rate equations, (2.17) and (2.18), using detailed balance between energy absorbed by the TS~ and energy lost by the phonons. For a single TS of energy E g(e)fipti=p1. Using (2.20) and (2.22) this can be written as defining a phonon scattering rate (3.2)  77y2,w A' tanh (E/k,T) pv: E2 (3.3) for the scattering of phonons of polarisation a by a single state with energy E and tunnel splitting A,. The total scattering at energy E is obtained by integrating over A. using f(a, A,) = PIA, (2.11) (noting that both +A and A contribute at a given E) which gives for the free path of a phonon of angular frequency w and polarisation cy. The thermal conductivity K( T) is evaluated on the assumption that heat is carried by nondispersive sound waves, consistent with the calculations leading to (2.26) and (3.4), and that scattering from TS dominates to give This gives general agreement with Lhe experimental results below 1 K both in respect of temperature dependence and magnitude, using the constant density of states derived from the heat capacity and a coupling constant y of order 1 ev. A more precise quantitative analysis requires information from acoustic experiments to separate longitudinal and transverse polarisation contributions in (3.6), and a more careful analysis of the heat capacity. Notice, however, that the interaction with phonons is dominated by TS with small asymmetry.
14 1670 W A Phillips Experimentally the temperature dependence is found to range from to T.9 indicating that the distribution function (2.11) is not strictly accurate. Eilack (1978) has pointed out that a distribution function of the form P(h) = P eua leads to K( T) proportional to TZPa, suggesting a width to the A distribution in the range This is not unreasonable, but the relatively small change in temperature depenldence shows the insensitivity of the calculation of K ( T) to the detailed form of the distribution functions. At higher temperatures the thermal conductivity passes through a plateau at temperatures between 4 and 20 K which has been explained in terms of increased scattering from a quadratically increasing density of TS (Zaitlin and Anderson 1975). Although there is some evidence from highfrequency acoustic measurements that the density of states may increase at higher energies (Pelous and Vacher 1976), it is extremely difficult to identify this contribution in the presence of relaxation scattering from the TS (3 4), higherorder phonon processes, structure scattering or even effects of phonon localisation Heat capacity The energy E and relaxation time T are more convenient parameters than A and A, when discussing heat capacity and other physical consequences of the distribution of tunnelling states. A distribution function (E, T) can be related to f(a, A,) by the Jacobian transformation This is a general result, but making use of the specific form f(a, A,) = P/Ao, D where P is the same constant that appears in 1;; (3.4) and T,~~(E), defined by replacing A, by E in (2.26), is the shortest relaxation time for states of energy E. The density of states is then given by integrating over all relaxation times from T, ~ up ~ to a value equal to the time scale to of the experiment: = $P ln(4t,/~,~~). The heat capacity can be calculated as in (1.1) to give m ~(t,) =;P 1n(4t,/~,,,) lo $$ sech ( ) 2kBT de (3.9) = &,rr2pkit ln(4t,/~,,,) (3.10) where the small energy variation of the logarithmic term, in the narrow range of E close to kbt which dominates the integral, has been neglected. Equation (3.10) encapsulates the nonequilibrium (nonergodic) nature of amorphous solids and not surprisingly has been the subject of numerous experimental
15 I I Twolevel states in glasses 1671 studies. Before examining the results on short time scales, it is helpful to assess the accuracy of (3.10) in respect of 'normal' measurements, where to is typically 10 s. Figure 6 shows C(T) in three samples of vitreous silica, Spectrosil B (about 1200ppm water), Suprasil (1000ppm water) and Suprasil W (almost no water). We will concentrate here on Suprasil W, where C( T) varies as T' in the range 25 mk < T < 250 mk, and where P = 3 x J' m3, yi = 1.6 ev and 7, = 1 ev can be deduced from K(T) and phonon echo experiments ( 3.1 and 5). The contribution of these states to C at 0.1 K can be calculated from (3.10) as 0.35 J kg' K' (taking to= 10 s and evaluating T,,, as 1 ps) in comparison to the experimental value of 0.7 J kg' K'. The logarithmic factor varies by 1.6 between 25 and 250 mk, giving a temperature variation approximately proportional to T' '. Bearing in mind a possible small energy dependence of P, the predicted temperature variation of C is in good agreement with experiment, although the magnitude is too small by a factor of two (Black 1978). This discrepancy could be ascribed to experimental uncertainties in the determination of yi and y, were it not for experiments at short time scales, which provide additional evidence that the reality is more complicated than that described by a single set of TS distributed according to (3.9). Such experiments are, however, notoriously Y  m m L al  h L. I I I I I I I 1 l l l l T IKI Figure 6. The heat capacity of 'waterfree' and 'wet' vitreous silica down to 25 mk. Also shown as a broken line is the Debye phonon contribution calculated from the velocities of sound (Lasjaunias et a[ 1975). 0, 0, Suprasil W (<1.5 ppmoh); 0, Suprasil (1200 ppm OH); A, Spectrosil B (1000 ppm OH) (Zeller and Pohl 1971).
16 1672 W A Phillips difficult (Goubau and Tait 1975, Kummer et a/ 1978, Lewis et a1 1978, Loponen et a/ 1980, 1982, Meissner and Spitzmann 1981). In general a short time scale is achieved by using thin samples of glass; at 0.4 K a sample 0.1 mm thick has a diffusion time of typically a few j ~ s. With a thin film heater on one side and a thermometer on the other the propagation of heat pulses through the sample can be followed to give either the diffusivity by fitting a diffusion equation to the measured temperature profile or the heat capacity by measuring the maximum temperature rise. One problem with this experimental arrangement is that even very thin metal films used as heaters or thermometers can have heat capacities comparable with the glass sample so that modelling thermal diffusion becomes difficult. There is limited agreement between the various experiments. Although all claim to see a timedependent heat capacity, the size of the effect differs greatly from one experiment to the next. The most consistent results are those of Meissner and Spitzmann (1981) (figure 7) and Loponen et a1 (1982) on Suprasil W, where the results tend to that predicted by (3.10) at time scales below 100 ps at temperatures below 1 K. For longer time scales C( t) changes more rapidly than expected, indicating another contribution to the heat capacity with a relatively well defined minimum relaxation time of about 100 ps at 0.3 K, and which when added to that derived from P gives approximate agreement with long time scale experiments below 1 K i Is) Figure 7. The measured heat capacity of vitreous silica as a function of the time scale of measurement at different temperatures: B 0.4 K; C, 0.6 K; E, 0.89 K; F, 1.0 K. The open circles represent the longtime data, and the broken lines the total heat capacity predicted by the tunnelling model. (Adapted from Meissner and Spitzmann (1981 ).)
Ordering, metastability and phase transitions in twodimensional systems
J. Phys. C: Solid State Phys., Vol. 6, 1973. Erinted in Great Britain. @ 1973 Ordering, metastability and phase transitions in twodimensional systems J M Kosterlit7 and D J Thouless Department of Mathematical
More informationSingleElectron Devices and Their Applications
SingleElectron Devices and Their Applications KONSTANTIN K. LIKHAREV, MEMBER, IEEE Invited Paper The goal of this paper is to review in brief the basic physics of singleelectron devices, as well as their
More informationManipulating atoms with photons*
Manipulating atoms with photons* Claude N. CohenTannoudji Collège de France et Laboratoire Kastler Brossel de l Ecole Normale Supérieure, 75231 Paris Cedex 05, France [S00346861(98)011039] Electromagnetic
More informationAcidbase Chemistry of Aquatic Systems
i Acidbase Chemistry of Aquatic Systems An introduction to the chemistry of acidbase equilibria with emphasis on the carbon dioxide system in natural waters eith A. Hunter Professor in Chemistry Department
More informationProperties of Electrons, their Interactions with Matter and Applications in Electron Microscopy
Properties of Electrons, their Interactions with Matter and Applications in Electron Microscopy By Frank Krumeich Laboratory of Inorganic Chemistry, ETH Zurich, VladimirPrelogWeg 1, 8093 Zurich, Switzerland
More informationSpaceTime Approach to NonRelativistic Quantum Mechanics
R. P. Feynman, Rev. of Mod. Phys., 20, 367 1948 SpaceTime Approach to NonRelativistic Quantum Mechanics R.P. Feynman Cornell University, Ithaca, New York Reprinted in Quantum Electrodynamics, edited
More informationScience, New Series, Vol. 220, No. 4598. (May 13, 1983), pp. 671680.
Optimization by Simulated Annealing S. Kirkpatrick; C. D. Gelatt; M. P. Vecchi Science, New Series, Vol. 220, No. 4598. (May 13, 1983), pp. 671680. Stable URL: http://links.jstor.org/sici?sici=00368075%2819830513%293%3a220%3a4598%3c671%3aobsa%3e2.0.co%3b28
More information1 OneDimensional Magnetism
1 OneDimensional Magnetism HansJürgen Mikeska 1 and Alexei K. Kolezhuk 1,2 1 Institut für Theoretische Physik, Universität Hannover, Appelstaße 2, 30167 Hannover, Germany, mikeska@itp.unihannover.de
More informationThe Scattering of α and β Particles by Matter and the Structure of the Atom
E. Rutherford, Philos. Mag, 6, 21 1911 The Scattering of α and β Particles by Matter and the Structure of the Atom E. Rutherford University of Manchester 1 (Received April 1911) 1 It is well known that
More informationOnedimensional wave turbulence
Physics Reports 398 (4) 65 www.elsevier.com/locate/physrep Onedimensional wave turbulence Vladimir Zakharov a;b,frederic Dias c;, Andrei Pushkarev d a Landau Institute for Theoretical Physics, Moscow,
More informationThermionic phenomena and the laws which govern them
OWEN W. RICHARDSON Thermionic phenomena and the laws which govern them Nobel Lecture, December 12, 1929 In its broadest aspect this subject may be summarized as the branch of Physics which deals with the
More informationControllability and Observability of Partial Differential Equations: Some results and open problems
Controllability and Observability of Partial Differential Equations: Some results and open problems Enrique ZUAZUA Departamento de Matemáticas Universidad Autónoma 2849 Madrid. Spain. enrique.zuazua@uam.es
More informationElectrowetting: from basics to applications
INSTITUTE OF PHYSICSPUBLISHING J.Phys.: Condens. Matter 17 (2005) R705 R774 JOURNAL OFPHYSICS: CONDENSED MATTER doi:10.1088/09538984/17/28/r01 TOPICAL REVIEW Electrowetting: from basics to applications
More informationRevisiting the Edge of Chaos: Evolving Cellular Automata to Perform Computations
Revisiting the Edge of Chaos: Evolving Cellular Automata to Perform Computations Melanie Mitchell 1, Peter T. Hraber 1, and James P. Crutchfield 2 In Complex Systems, 7:8913, 1993 Abstract We present
More informationLearning Objectives for AP Physics
Learning Objectives for AP Physics These course objectives are intended to elaborate on the content outline for Physics B and Physics C found in the AP Physics Course Description. In addition to the five
More informationA Molecular Dynamics Study of Slow Base Flipping in DNA using Conformational Flooding
770 Biophysical Journal Volume 93 August 2007 770 786 A Molecular Dynamics Study of Slow Base Flipping in DNA using Conformational Flooding Benjamin Bouvier and Helmut Grubmüller Theoretical and Computational
More informationDistinctive Image Features from ScaleInvariant Keypoints
Distinctive Image Features from ScaleInvariant Keypoints David G. Lowe Computer Science Department University of British Columbia Vancouver, B.C., Canada lowe@cs.ubc.ca January 5, 2004 Abstract This paper
More informationAbout the Author. journals as Physics Letters, Nuclear Physics and The Physical Review.
About the Author Dr. John Hagelin is Professor of Physics and Director of the Doctoral Program in Physics at Maharishi International University. Dr. Hagelin received his A.B. Summa Cum Laude from Dartmouth
More information32. Passage of particles through matter 1
32. Passage of particles through matter 1 32. PASSAGE OF PARTICLES THROUGH MATTER...................... 2 32.1. Notation.................... 2 32.2. Electronic energy loss by heavy particles...... 2 32.2.1.
More informationON THE DISTRIBUTION OF SPACINGS BETWEEN ZEROS OF THE ZETA FUNCTION. A. M. Odlyzko AT&T Bell Laboratories Murray Hill, New Jersey ABSTRACT
ON THE DISTRIBUTION OF SPACINGS BETWEEN ZEROS OF THE ZETA FUNCTION A. M. Odlyzko AT&T Bell Laboratories Murray Hill, New Jersey ABSTRACT A numerical study of the distribution of spacings between zeros
More informationUnderstanding the FiniteDifference TimeDomain Method. John B. Schneider
Understanding the FiniteDifference TimeDomain Method John B. Schneider June, 015 ii Contents 1 Numeric Artifacts 7 1.1 Introduction...................................... 7 1. Finite Precision....................................
More informationTwodimensional turbulence: a physicist approach
Physics Reports 362 (2002) 1 62 Twodimensional turbulence: a physicist approach PatrickTabeling Laboratoire de Physique Statistique, Ecole Normale Superieure, 24 rue Lhomond, 75231 Paris, France Received
More informationOn the Constitution of Atoms and Molecules. N. Bohr, Dr. phil. Copenhagen (Received July 1913)
N. Bohr, Philos. Mag. 26, 1 1913 Introduction On the Constitution of Atoms and Molecules N. Bohr, Dr. phil. Copenhagen (Received July 1913) In order to explain the results of experiments on scattering
More informationFlow at. Experiments on TwoDimensional Base Subsonic and Transonic Speeds MINISTRY OF AVIATION ~0 L~AL AIRCP, A ~':T... R. & M. No.
R. & M. No. 3427 ~0 L~AL AIRCP, A ~':T... MINISTRY OF AVIATION AERONAUTICAL RESEARCH COUNCIL REPORTS AND MEMORANDA Experiments on TwoDimensional Base Subsonic and Transonic Speeds Flow at By J. F. NASH,
More informationTHE PROBLEM OF finding localized energy solutions
600 IEEE TRANSACTIONS ON SIGNAL PROCESSING, VOL. 45, NO. 3, MARCH 1997 Sparse Signal Reconstruction from Limited Data Using FOCUSS: A Reweighted Minimum Norm Algorithm Irina F. Gorodnitsky, Member, IEEE,
More informationThe predictability of a flow which possesses many scales of motion
The predictability of a flow which possesses many scales of motion By EDWARD N. LORENZ, Massachusetts Institute of Technology1 (Manuscript received October 31, 1968, revised version December 13, 1968)
More informationTimeCorrelated Single Photon Counting
Technical Note TimeCorrelated Single Photon Counting Michael Wahl PicoQuant GmbH, Rudower Chaussee 29, 12489 Berlin, Germany, info@picoquant.com The Principle of TimeCorrelated Single Photon Counting
More informationTISSUE INHOMOGENEITY CORRECTIONS FOR MEGAVOLTAGE PHOTON BEAMS
AAPM REPORT NO. 85 TISSUE INHOMOGENEITY CORRECTIONS FOR MEGAVOLTAGE PHOTON BEAMS Report of Task Group No. 65 of the Radiation Therapy Committee of the American Association of Physicists in Medicine Members
More informationThe Climate System: an Overview
1 The Climate System: an Overview Coordinating Lead Author A.P.M. Baede Lead Authors E. Ahlonsou, Y. Ding, D. Schimel Review Editors B. Bolin, S. Pollonais Contents 1.1 Introduction to the Climate System
More informationOn Graphite Transformations at High Temperature and Pressure Induced by Absorption of the LHC Beam
LHC Project Note 78 / 97 January 18, 1997 zazula@mail.cern.ch On Graphite Transformations at High Temperature and Pressure Induced by Absorption of the LHC Beam Jan M. Zazula CERNSL/BT(TA) Keywords: Summary
More information